Published on Web 06/23/2007
Magnetic Core/Shell Fe3O4/Au and Fe3O4/Au/Ag Nanoparticles with Tunable Plasmonic Properties Zhichuan Xu, Yanglong Hou, and Shouheng Sun* Department of Chemistry, Brown UniVersity, ProVidence, Rhode Island 02912 Received May 1, 2007; E-mail: [email protected]
Synthesis of magnetic nanoparticles has long been of scientific and technological interest due to their potential applications in tissue imaging,1 drug delivery,2 and information storage.3 Important progress has been made in chemical synthesis of monodisperse magnetic nanoparticles of metals,4 alloys,3b and oxides.5 Recently, incorporation of optically active components onto magnetic nanoparticles has attracted much attention. Dumbbell-like Au-Fe3O46 or CdS-FePt7 nanoparticles have been synthesized and shown interesting optical properties in Au or CdS and magnetic properties in Fe3O4 or FePt. Au coating over magnetic nanoparticles is an even more attractive composite system:8,9 with Au coating, the magnetic nanoparticles, especially high moment metallic magnetic nanoparticles, can be stabilized more efficiently in corrosive biological conditions and readily functionalized through the welldeveloped Au-S chemistry; the coating also renders the magnetic nanoparticles with plasmonic properties. This makes the core/shell composite nanoparticles extremely interesting for magnetic, optical, and biomedical applications. Here we present a facile synthesis of Au- and Ag-coated Fe3O4 nanoparticles with controlled plasmonic and magnetic properties. The synthesis starts with room temperature coating of Au on the surface of Fe3O4 nanoparticles by reducing HAuCl4 in a chloroform solution of oleylamine. The Au-coated Fe3O4 nanoparticles are then transferred into water by mixing them with sodium citrate and cetyltrimethylammonium bromide (CTAB). The water-soluble core/ shell Fe3O4/Au nanoparticles serve as seeds for the formation of Fe3O4/Au nanoparticles with thicker Au coating by simply adding more HAuCl4 in the reducing condition or for the preparation of Fe3O4/Au/Ag nanoparticles by adding AgNO3 to the reaction mixture. The plasmonic properties of these core/shell nanoparticles can be tuned by controlling the coating thickness and coating materials. Our synthesis is fundamentally different from the previous methods in synthesizing Au- and Ag-coated magnetic nanoparticles in aqueous8 and organic solutions9 and achieves the uniform coating of Au and Ag on monodisperse Fe3O4 nanoparticles. The mild synthetic conditions reported here will also allow the synthesis of core/shell Fe3O4/Au with different shapes, facilitating the tuning of plasmonic properties in a wide range of spectrum.10 The oleylamine and oleic acid capped 10 nm Fe3O4 nanoparticles were synthesized via thermal decomposition of iron(III) oleate in a mixture of oleylamine and oleic acid11,12 and were used for the synthesis of Fe3O4/Au nanoparticles. Figure 1A outlines the synthesis: 10 nm Fe3O4 nanoparticles (i) were first coated with a thin layer of Au to make Fe3O4/Au (ii). The coating experiment was carried out by gently reducing hydrogen tetrachloroaurate hydrate (HAuCl4‚3H2O) in a chloroform solution of oleylamine in the presence of (i).12 Oleylamine was used as a mild reducing agent as well as a surfactant. The as-prepared core/shell nanoparticles (ii) dispersed well in nonpolar solvent. To make water-soluble core/ shell nanoparticles (iii), the dry hydrophobic nanoparticles (ii) were dissolved in an aqueous solution containing 0.1 M CTAB and 0.1 8698
J. AM. CHEM. SOC. 2007, 129, 8698-8699
Figure 1. (A) Schematic illustration of surface coating of Fe3O4 nanoparticles (i) with Au to form hydrophobic Fe3O4/Au nanoparticles (ii) and hydrophilic Fe3O4/Au nanoparticles (iii). (B) TEM image of the nanoparticles (iii); (C) HRTEM image of part of a single Fe3O4/Au nanoparticle from (B). (D) UV-vis absorption spectra of the nanoparticles (i) in hexane, (ii) in hexane, and (iii) in water.
mM sodium citrate. It is well-known that sodium citrate can attach to Au and provides a negatively charged surface for Au nanoparticle stabilization.13 However, our test showed that sodium citrate alone could not stabilize Fe3O4/Au nanoparticles in water. Combined CTAB, a cationic surfactant, with citrate, and the Fe3O4/Au nanoparticles were well-stabilized due to the formation of a CTAB double layer on the nanoparticle surface.10a,b The core/shell Fe3O4/ Au nanoparticles (iii) capped with citrate-CTAB were readily dispersed in water, forming a light pink colloidal solution.12 The same CTAB/citrate method could be applied to dissolve oleylamine capped Au nanoparticles into water, but not Fe3O4 nanoparticles, indicating that the as-prepared core/shell nanoparticles are coated with Au. Transmission electron microscope (TEM) analysis on both Fe3O4 and Fe3O4/Au nanoparticles reveals that the overall inorganic diameter is increased from 10 nm of the as-synthesized Fe3O4 nanoparticles to ∼12 nm of the Fe3O4/Au (iii) nanoparticles. Figure 1B is the TEM image of core/shell nanoparticles (iii), and Figure 1C shows the high-resolution TEM (HRTEM) of a single Fe3O4/ Au nanoparticle. The lattice fringes in the Au shell are clearly seen in the HRTEM, and the interfringe spacing is 0.201 nm, close to the interplane distance of the (200) planes in the face centered cubic (fcc) Au, indicating the Fe3O4 nanoparticles are coated with a layer (∼1 nm) of crystalline Au.12 UV-vis absorption of the assynthesized Fe3O4 nanoparticles (i) and the core/shell nanoparticles [(ii) and (iii)] shows different absorption properties as shown in Figure 1D. The core/shell nanoparticles (ii) dispersed in hexane have a similar spectrum to that from (i). Once capped with citrate and CTAB, the nanoparticles (iii) show an absorption band at 534 nm. Clearly, this optical property change is caused by the change of surface charge. It is known that the surface plasmon for the small Au nanoparticles has a strong absorption when the surface of the particles is charged, while no surface plasmon is observed when 10.1021/ja073057v CCC: $37.00 © 2007 American Chemical Society
function of the Au/Ag shell toward Ag15 and thus the shift of the absorption peak from 534 to 501 nm. Note that the thickness increase in the Au or Ag shell results in the decrease in magnetic moment of the core/shell nanoparticles due to the weight contribution from the nonmagnetic Au and Ag.12 We have shown that the core/shell structured Fe3O4/Au and Fe3O4/Au/Ag nanoparticles can be readily synthesized in aqueous solution and room temperature reaction conditions. The control on shell thickness allows the tuning of plasmonic properties of the core/shell nanoparticles to be either red-shifted (to 560 nm) or blueshifted (to 501 nm). The significant contribution of the synthesis is that it offers not only a composite nanoparticle system with controlled magnetic and plasmonic properties but also a noble metalcoated surface for long-term stabilization of the magnetic core and nanoparticle functionalization. Such multifunctional nanoparticles should have great potentials for nanoparticle-based diagnostic and therapeutic applications. Acknowledgment. This work was supported by Salomon award from Brown University, the Frontier Research Award from the Department of Chemistry, Brown University, and by NSF/DMR 0606264. Figure 2. (A) Schematic illustration of the formation of Fe3O4/Au and Fe3O4/Au/Ag and the control on the plasmonic properties; (B) XRD of the Fe3O4/Au nanoparticles with various Au coating thickness; (C) UV-vis absorption spectra of the core/shell Fe3O4/Au and Fe3O4/Au/Ag nanoparticles with various Au and Ag coating thickness.
the surface of these nanoparticles is protected by a long alkyl chain ligand in nonpolar solvent.14 The charge density on the surface of the core/shell nanoparticles (iii) and the amplitude of the free electron oscillation within the particles are significantly increased due to the coating with citrate and CTAB, leading to enhanced plasmonic absorption. Core/shell Fe3O4/Au nanoparticles (iii) can be used as seeds for continued growth of Au shell or Ag shell, as illustrated in Figure 2A. The deposition of Au or Ag was carried out by reducing HAuCl4 or AgNO3 using ascorbic acid in the presence of CTAB.12 This reduction chemistry has been found to be effective in making a uniform coating layer on gold nanorods.10 The coating thickness was controlled by the amount of HAuCl4 or AgNO3 present in the reaction mixture. Figure 2B gives a series of X-ray diffraction (XRD) patterns of the Fe3O4/Au nanoparticles with various Au coating thickness. The evolution of the diffraction peaks from fcc Au is clearly seen in the patterns. As Au coating thickness increases, the diffraction from Au dominates the patternsat 2.5 nm coating, the diffraction from Fe3O4 is too weak to be detected due to the heavy atom effect of Au. TEM image analyses on both Fe3O4/Au and Fe3O4/Au/Ag nanoparticles indicate the increase of the overall diameter of the particles compared to the as-synthesized Fe3O4 nanoparticles,12 proving the coating control in the synthesis. The controlled coating of either Au or Ag on the Fe3O4/Au nanoparticles (iii) facilitates the tuning of plasmonic properties of these core/shell nanoparticles. Figure 2C lists a series of UV-vis spectra from Fe3O4/Au and Fe3O4/Au/Ag nanoparticles in aqueous dispersions. The starting Fe3O4/Au nanoparticles (iii) have an absorption peak at 534 nm. Depositing more Au on the nanoparticles leads to a red-shift of the absorption peak, while coating Ag on (iii) results in a blue-shift of the spectrum. The absorption band can be red-shifted to 561 nm by increasing the thickness of the Au shell to ∼3 nm or blue-shifted to 501 nm by coating 2 nm Ag on (iii). The deposition of Ag on Au changes the effective dielectric
Supporting Information Available: Experimental and characterization details. This material is available free of charge via the Internet at http://pubs.acs.org. References (1) (a) Lee, J. H.; Huh, Y. M.; Jun, Y. W.; Seo, J. W.; Jang, J. T.; Song, H. T.; Kim, S. J.; Cho, E. J.; Yoon, H. G.; Suh, J. S.; Cheon, J. W. Nat. Med. 2007, 13, 95. (b) Seo, W. S.; Lee, J. H.; Sun, X. M.; Suzuki, Y.; Mann, D.; Liu, Z.; Terashima, M.; Yang, P. C.; Mcconnell, M. V.; Nishimura, D. G.; Dai, H. J. Nat. Mater. 2006, 5, 971. (2) (a) Son, S. J.; Reichel, J.; He, B.; Schuchman, M.; Lee, S. B. J. Am. Chem. Soc. 2005, 127, 7316. (b) Zhao, W.; Gu, J.; Zhang, L.; Chen, H.; Shi, J. J. Am. Chem. Soc. 2005, 127 8916. (3) (a) Majetich, S. A.; Jin, Y. Science 1999, 284, 470. (b) Sun, S. H.; Murray, C. B.; Weller, D.; Folks, L.; Moser, A. Science 2000, 287, 1989. (4) Murray, C. B.; Sun, S. H.; Doyle, H.; Betley, T. MRS Bull. 2001, 26, 985. (5) Sun, S. H.; Zeng, H.; Robinson, D. B.; Raoux, S.; Rice, P. M.; Wang, S. X.; Li, G. X. J. Am. Chem. Soc. 2004, 126, 273. (6) (a) Yu, H.; Chen, M.; Rice, P. M.; Wang, S. X.; White, R. L.; Sun, S. H. Nano Lett. 2005, 5, 379. (b) Li, Y. Q.; Zhang, Q.; Nurmikko, A. V.; Sun, S. Nano Lett. 2005, 5, 1689. (7) (a) Gu, H. W.; Zheng, R. K.; Zhang, X. X.; Xu, B. J. Am. Chem. Soc. 2004, 126, 5664. (b) Gu, H. W.; Yang, Z. M.; Gao, J. H.; Chang, C. K.; Xu, B. J. Am. Chem. Soc. 2005, 127, 34. (8) (a) Lin, J.; Zhou, W.; Kumbhar, A.; Wiemann, J.; Fang, J.; Carpenter, E. E.; O’Connor, C. J. J. Solid State Chem. 2001, 159, 26. (b) Cho, S. J.; Idrobo, J. C.; Olamit, J.; Liu, K.; Browning, N. D.; Kauzlarich, S. M. Chem. Mater. 2005, 17, 3181. (c) Mikhaylova, M.; Kim, D. K.; Bobrysheva, N.; Osmolowsky, M.; Semenov, V.; Tsakalatos, T.; Muhammed, M. Langmuir 2004, 20, 2472. (d) Mandal, M.; Kundu, S.; Ghosh, S. K.; Panigrahi, S.; Sau, T. K.; Yusuf, S. M.; Pal, T. J. Colloid Interface Sci. 2005, 286, 187. (e) Lyon, J. L.; Fleming, D. A.; Stone, M. B.; Schiffer, P.; Williams, M. E. Nano Lett. 2004, 4, 719. (9) (a) Wang, L. Y.; Luo, J.; Fan, Q.; Suzuki, M.; Suzuki, I. S.; Engelhard, M. H.; Lin, Y. H.; Kim, N.; Wang, J. Q.; Zhong, C. J. J. Phys. Chem. B 2005, 109, 21593. (b) Wang, L. Y.; Luo, J.; Maye, M. M.; Fan, Q.; Rendeng, Q.; Engelhard, M. H.; Wang, C. M.; Lin, Y. H.; Zhong, C. J. J. Mater. Chem. 2005, 15, 1821. (10) (a) Nikoobakht, B.; El-Sayed, M. A. Chem. Mater. 2003, 15, 1957. (b) Gao, J. X.; Bender, C. M.; Murphy, C. J. Langmuir 2003, 19, 9065. (c) Liu, M. Z.; Guyot-Sionnest, P. J. Phys. Chem. B 2004, 108, 5882. (11) Park, J. N.; An, K. J.; Hwang, Y. S.; Park, J. G.; Noh, H. J.; Kim, J. Y.; Park, J. H.; Hwang, N. M.; Hyeon, T. W. Nat. Mater. 2004, 3, 891. (12) Supporting Information. (13) (a) Frens, G. Nat. Phys. Sci. 1973, 241, 20. (b) Sutherland, W. S.; Winefordner, J. D. J. Colloid Interface Sci. 1992, 48, 129. (14) (a) Lica, G. C.; Zelakiewicz, B. S.; Constantinescu, M.; Tong, Y. Y. J. Phys. Chem. B 2004, 108, 19896. (b) Kreibig, U.; Frauth, K.; Granqvist, C. G.; Schmid, G. Z. Phys. Chem. 1990, 169, 11. (15) Liu, M. Z.; Guyot-Sionnest, P. J. Phys. Chem. B 2004, 108, 5882.
J. AM. CHEM. SOC.
VOL. 129, NO. 28, 2007 8699